#------------------------------------------------------------------------------
#$Date: 2014-08-15 21:14:22 +0300 (Fri, 15 Aug 2014) $
#$Revision: 23 $
#$URL: svn+ssh://sauliusg@svn.code.sf.net/p/propcif/code/trunk/cif/1/1000112.mpod $
#------------------------------------------------------------------------------
#
# This file is available in the Material Properties Open Database (MPOD),
# http://www.materialproperties.org/
#
# The file may be used within the scientific community so long as
# proper attribution is given to the journal article from which the
# data were obtained.
#
data_1000112
_cod_database_code ?
_structure_refined 'no'
_mpod_phase_name '?'
_chemical_formula_moiety LaRu2P2
_chemical_formula_sum 'La Ru2 P2'
_mpod_symmetry_point_group_name_H-M '?'
_cell_length_a  ?
_cell_length_b  ?
_cell_length_c  10.67
_cell_angle_alpha  90
_cell_angle_beta   90
_cell_angle_gamma  90
loop_
_publ_author_name
'Ying, J.J.'
'Yan, Y.J.'
'Liu, R.H.'
'Wang, X.F.'
'Wang, A.F.'
'Zhang, M.'
'Xiang, Z.J.'
'Chen, X.H.'
_publ_section_title
;
 Isotropic superconductivity in LaRu2P2 with the ThCr2Si2-type structure
;
_journal_name_full               'Superconductor Science and Technology'
_journal_volume                  23
_journal_issue                   10
_journal_article_reference       115009
_journal_pages_number            4
_journal_year                    2010
_mpod_phase_density ?
_prop_measurement_method '?'
_prop_conditions_magnetic_field ?
_prop_electric_resistivity_rhoeij 'rhoeij'
_prop_superconducting_critical_temperature_onset ?
_prop_superconducting_critical_temperature_onset_90 ?
_prop_superconducting_critical_temperature_mid_50 3.7
_prop_superconducting_critical_temperature_offset_10 ?
_prop_superconducting_critical_temperature_thermodynamic ?
_prop_superconducting_zero_resistivity_temperature ?
_prop_superconducting_resistivity_transition_width 0.1
_prop_superconducting_critical_field2_Hc2i 'Hc2i'
_prop_superconducting_critical_field1_Hc1i 'Hc1i'
_prop_superconducting_irreversibility_field_Hirri 'Hirri'
_prop_superconducting_coherence_length_ksii 'ksii'
_prop_superconducting_penetration_depth_lambdai 'lambdai'
_prop_residual_resistivity_ratio 12.4
_prop_residual_resistivity_ratio_high_temperature 300
_prop_residual_resistivity_ratio_low_temperature 4
loop_
_prop_data_label
_prop_data_tensorial_index
_prop_data_value
_prop_conditions_temperature
rhoeij 11 110 300
rhoeij 22 110 300
rhoeij 33 ? ?
rhoeij 11 8.9 4
rhoeij 22 8.9 4
rhoeij 33 ? ?
Hc1i 1 0.023 0
Hc1i 2 0.023 0
Hc1i 3 0.023 0
Hc1i 1 0.0114 1.8
Hc1i 2 0.0114 1.8
Hc1i 3 0.0100 1.8
Hc2i 1 0.114 0
Hc2i 2 0.114 0
Hc2i 3 0.114 0
Hirri 1 0.055 1.8
Hirri 2 0.055 1.8
Hirri 3 0.0544 1.8
ksii 1 54 0
ksii 2 54 0
ksii 3 54 0
lambdai 1 80 0
lambdai 2 80 0
lambdai 3 80 0
